Molecular Hydrogen Formation from Proximal Glycol Pairs on TiO2(110) Long Chen, Zhenjun Li,† R. Scott Smith, Bruce D. Kay, and Zdenek Dohnálek* Fundamental and Computational Sciences Directorate and Institute for Integrated Catalysis, Paciﬁc Northwest National Laboratory, P.O. Box 999, Richland, Washington 99352, United States S Supporting Information *
another HOb group.9−13 Upon heating to ∼500 K, the resulting HOb’s recombine with another HOb or an alkoxy to produce a water or an alcohol molecule, respectively.14−18 For alcohols, the majority of alkoxy species (except for methanol which recombinatively desorbs) undergo dehydration to alkenes and water.15−18 As a consequence, molecular hydrogen desorption from alcohols and water on TiO2(110) has not been generally observed.15−21 In line with these observations, theoretical calculations demonstrate that the kinetic barrier for H2 recombinative desorption from HOb sites on TiO2(110) is considerably higher than the barrier for water formation.20,21 However, in a recent temperature-programmed desorption (TPD) study,22 Xu et al. reported that D2 is formed as a minor product via thermal recombination of the D atoms on Ob sites from photocatalysis of methanol. Interestingly, hydrogen desorption between 375 and 500 K was also observed in our recent study of ethylene glycol (EG) reactions on TiO2(110).23 Molecular hydrogen evolution from EG on TiO2(110) was ﬁrst observed in a study of ethanol, n- and 2-propanol, EG, and diethyl ether via TPD and X-ray photoelectron spectroscopy (XPS).24 Subsequent detailed quantitative investigations with diﬀerent isotopes (i.e., HO(CH2)2OH, DO(CH2)2OD, and HO(CD2)2OH) demonstrated that the observed hydrogen originates solely from hydroxyl groups and that high EG coverages are required for its formation.23 While at low coverages, ethylene and water were identiﬁed as the only products, at saturation coverage both ethylene + water and acetaldehyde + hydrogen were observed. Total product yield of carbon-containing products at saturation coverage was determined to be ∼0.5 monolayer (ML), which clearly shows that the reactions proceed not only at VO defect sites but also on the Ti5c rows. In this study, we systematically investigate hydrogen formation from a series of glycols with diﬀerent steric constraints on diﬀerently prepared TiO2(110) surfaces in order to further understand hydrogen formation from glycols, and polyols in general. We ﬁnd that hydrogen formation is dramatically attenuated for glycols with methyl end-groups shielding the hydroxyl functional groups. Further, hydrogen formation is not observed on disordered or oxidized TiO2(110). These results suggest that on TiO2(110), pairs of aligned glycol molecules with hydroxyl groups in close proximity, together with subsurface charge are required to carry out this redox reaction.
ABSTRACT: Understanding hydrogen formation on TiO2 surfaces is of great importance, as it could provide fundamental insight into water splitting for hydrogen production using solar energy. In this work, hydrogen formation from glycols having diﬀerent numbers of methyl end-groups has been studied using temperature-programmed desorption on reduced, hydroxylated, and oxidized rutile TiO2(110) surfaces. The results from OD-labeled glycols demonstrate that gas-phase molecular hydrogen originates exclusively from glycol hydroxyl groups. The yield is controlled by a combination of glycol coverage, steric hindrance, TiO2(110) order, and the amount of subsurface charge. Combined, these results show that proximal pairs of hydroxyl-aligned glycol molecules and subsurface charge are required to maximize the yield of this redox reaction. These ﬁndings highlight the importance of geometric and electronic eﬀects in hydrogen formation from adsorbates on TiO2(110).
he technological importance of TiO2 has driven cuttingedge research with the aim of understanding the elementary steps that underlie catalytic and photocatalytic reactions on this material.1−5 In this context hydrogen, as a promising source of clean, renewable, and environmentally friendly energy, is of great interest.2,6−8 As such, understanding the factors that control its formation in the thermal and photocatalytic conversion of water and organics is of critical importance. While a signiﬁcant eﬀort has been devoted to this subject, the mechanism of hydrogen formation on TiO2 is far from understood. For catalytic and photocatalytic studies in particular, the most stable TiO2 surface, rutile TiO2(110), has served as a prototypical model.4,5 When stoichiometric or slightly reduced, the surface is unreconstructed and composed of alternating 5fold-coordinated Ti4+ (Ti5c) and bridging oxygen (Ob) rows. A small fraction of bridging oxygen vacancy defects (VO’s) that form as a consequence of TiO2 bulk reduction during ultrahigh vacuum (UHV) preparation, play an important role in determining the surface reactivity of TiO2(110).1,4 Water and alcohols have been thoroughly investigated on TiO2(110) due to their importance as models in studies of photocatalytic water splitting and photo-oxidation of organic contaminants.1−5 Both water and alcohol molecules initially dissociate at a VO site ﬁlling it with a hydroxy (HOb) and/or alkoxy group, respectively, and splitting hydrogen that forms © 2014 American Chemical Society
Received: January 28, 2014 Published: April 4, 2014 5559
dx.doi.org/10.1021/ja500992b | J. Am. Chem. Soc. 2014, 136, 5559−5562
Journal of the American Chemical Society
The experiments were carried out in a UHV molecular beam surface scattering apparatus (base pressure < 7 × 10−11 Torr) described previously.16,25 A rutile TiO2(110) crystal (10 × 10 × 1 mm3, Princeton Scientiﬁc) was cleaned by cycles of Ne+ sputtering and annealing to 850−900 K in UHV until impurities were undetectable in Auger electron spectra. The surface prepared in this way (referred to as r-TiO2(110)) contained ∼5% VO defects as determined by H2O TPD.14,26 Additionally, hydroxylated (h-TiO2(110)) and oxidized (oTiO2(110)) surfaces were prepared by exposing r-TiO2(110) to D2O at 400 K, and to O2 at 70 K, followed by annealing to 300 K, respectively.27,28 All glycols (ethylene glycol, 1,2- and 1,3propylene glycols, 2,3-butylene glycol, 2,3-dimethyl-2,3-butylene glycol) used in this study were obtained from SigmaAldrich and transferred into ﬂasks with baked molecular sieves. The glycols were puriﬁed by pumping at room temperature, and their temperature during the dose was stabilized in a water bath. The glycols were dosed onto the various TiO2(110) surfaces using an eﬀusive molecular beam. TPD measurements (ramp rate of 1 K/s) were performed using a quadrupole mass spectrometer (UTI). To unambiguously determine the origin of hydrogen (O−H vs C−H), we employ OD-labeled glycols and monitor the D2 signal during the TPD experiments. Since not all OD-labeled glycols are commercially available we prepared them directly on TiO2(110) using an H/D exchange procedure as described in the Supporting Information (SI). The viability of this procedure has been conﬁrmed by comparing the TPD spectra from the isotopically exchanged 1,2-propylene glycol (1,2-PG) with those of commercially available OD-labeled 1,2-PG (Figure S1, SI). The use of OD-labeled glycols further allows us to overcome the experimental diﬃculties associated with high H2 background during TPD due to H2 desorption from a closedcycle He-cryostat cooled manipulator.23 Figure 1a shows the coverage-dependent D2 TPD spectra from OD-labeled ethylene glycol (DO(CH2)2OD), 1,3propylene glycol (DO(CH2)3OD), 1,2-propylene glycol (DOCH2CH(CH3)OD), 2,3-butylene glycol (DOCH(CH3)CH(CH3)OD), and 2,3-dimethyl-2,3-butylene glycol (DOC(CH3)2C(CH3)2OD) on r-TiO2(110). Other products include water and a broad range of carbon-containing species. While the discussion of the carbon-containing products for all employed glycols is beyond the scope of this report, generally alkenes are observed at low coverages, and both alkenes and aldehydes/ketones are seen at high coverages. For EG, all the products and their coverage dependences were discussed in detail in our prior publication23 and are also summarized in Figure S2 in SI. Further, since D2 desorption occurs at lower temperatures than desorption of any carbon-containing products (see data for EG23 in Figure S2, SI), we believe that D2 formation is largely decoupled from the formation of carbon-containing products at higher temperatures. The selected sequence of glycol molecules allows us to explore how the methyl end-groups that surround the hydroxyl functional groups aﬀect D2 formation. Figure 1a shows that for each glycol molecule. With the exception of 2,3-dimethyl-2,3butylene glycol, the amount of desorbing D2 is strongly dependent on the coverage. While at low coverages (